# Epsilon Paper

### Transcript of Epsilon Paper

Critical Assessment: Martensite–Start Temperature

for the γ → ε Transformation

H.-S. Yang*, J. H. Jang*, H. K. D. H. Bhadeshia*† and D. W. Suh*

*Graduate Institute of Ferrous Technology (GIFT)Pohang University of Science and Technology (POSTECH)

Pohang 790-784, Republic of Korea

†University of CambridgeMaterials Science and Metallurgy

Pembroke Street, Cambridge CB2 3QZ, U. K.

Abstract

It is increasingly important in the context of high–manganese steels of the kind that lead totwinning–induced plasticity to be able to estimate the temperature at which ε–martensite formswhen austenite is cooled. We find that the thermodynamic method used in similar calculations forα′ martensite cannot in many cases be implemented because of apparently imprecise thermody-namic data, a conclusion partly validated using limited first–principles calculations. Alternative,empirical methods are also evaluated. The austenite grain size dependence of the martensite–starttemperature has also been rationalised in terms of existing theory for α′ martensite. Experimentshave also been conducted to show that the problem in dealing with the ε–martensite does not liein the precision with which the transformation can be measured using dilatometry.

Keywords: Martensite; thermodynamics; epsilon; start temperature; high Mn steels

1 Introduction

The basis for the calculation of the martensite–start (MS) temperature was reviewed some time agoby Kaufman and Cohen [1]; martensite is triggered when the free energy change for transformation

without a composition change (∆Gγα′

) reaches a critical value (∆Gγα′

MS), the magnitude of which

is determined by stored energies and kinetic phenomena [2, 3]. Here γ refers to austenite and α′

to body–centred cubic or body–centred tetragonal martensite. The method has been applied withsome success to the γ → α′ transformation [4–12] and forms the basis of computer programs whichtake as inputs the thermodynamic parameters of the parent and product phases and output the

1

CALPHAD 36 (2012) 16-22

transformation–start temperature (for example, [13]). In this way, the incorporation of a previouslyexcluded element on the MS temperature simply requires an understanding of how this elementalters the thermodynamic stabilities of the phases involved.

Iron in which the atoms are arranged on a hexagonal lattice is designated ε. Although this is nota common allotrope in alloyed iron at ambient pressure, it is gaining importance in low–carbon,often low density, structural steels containing unconventionally large concentrations of manganese[14–16]. It is also the basis of many iron–based shape memory alloys [17–19]. The ε thereforefeatures in reversible martensitic transformations and in steels where its transformation plasticityis exploited. It is important therefore, in the process of alloy design and optimisation, to be ableto calculate its martensite–start temperature, at least as a function of the chemical composition.

The last attempt at dealing with this issue was by Dogan and Ozer [20] who derived an empiricalequation using linear regression analysis on some 17 iron–based alloys which undergo the γ → ǫmartensitic transformation as follows:

MS/K = 246− 5.8wMn + 38.5wSi − 61.5wCr − 5.1wNi + 138wCe − 146wTi − 396wN (1)

where w represents the weight percent of the element identified in the subscript. The equation wasderived for the concentration ranges 13.0–31.5Mn, 4.7–7.0Si, 0–11.6Cr, 0–6.8Ni wt%; Ce, Ti and Nwere each present in single alloys with values of 0.3, 0.6 and 0.3wt% respectively. Standard errorswere not quoted but the deviation from a fit to this equation were typically less than ±20◦C.

Dogan and Ozer also considered the use of thermodynamics as described above; however, neitherthe origin of the thermodynamic data nor the calculations of MS temperatures were presented inthe paper, so it is not clear what was achieved. The purpose of the present work was to take afresh look at this problem given the much larger availability of data due to the increased moderninterest in low density and TRIP (transformation induced plasticity) steels based on the ε phase.To achieve this we have used a variety of empirical, thermodynamic and first–principles techniques.

2 Data

A search of the literature revealed a large number of sources of data [20–78] which yielded some328 combinations of chemical composition and martensite–start temperatures. The properties ofthe data are summarised in Table 1, and a spreadsheet containing the full details is available on[79]. The elements included C, Mn, Ni, Cr, Al, Si, Mo, Co, Cu, Nb, Ti, V and W.

The data were subjected to multiple regression analysis to yield the following relationship whichhas a standard error of ±26K and a correlation coefficient of 0.9:

MS/K = 576 ± 8− (489 ± 31)wC − (9.1 ± 0.4)wMn − (17.6 ± 2)wNi − (9.2 ± 1)wCr+(21.3 ± 2)wAl + (4.1± 1)wSi − (19.4 ± 5)wMo − (1± 1)wCo − (41.3 ± 6)wCu−(50± 18)wNb − (86± 12)wTi − (34± 10)wV − (13± 5)wW (2)

The extent of the fit is illustrated in Fig. 1 and forms a rough method of estimating the martensite–start temperature but the linear relationship and the implied lack of dependences between the

2

independent variables clearly cannot be justified. These particular issues are tackled later in thetext when describing the neural network method, but a more fundamental approach would involvecalculations based on phase stabilities which we address next.

3 Thermodynamic Calculations

By analogy with the transformation of austenite into α′ martensite described in the introduction,the martensite–start temperature for ε–martensite corresponds to that at which the driving force∆Gγε achieves a critical value ∆Gγε

MS. Values of the driving force can in principle be calculated

using standard thermodynamic databases in combination with programs such as ThermoCalc orMTDATA. In the present work we used the TCFE6 database and ThermoCalc to produce theresults illustrated in Fig. 2, which shows ∆Gγε

MSas a function of the measured transformation–start

temperatures obtained from the literature. The results are worrying in two respects; first, thatthe driving force for a large number of alloys is positive, i.e., it is thermodynamically impossiblefor ε to form even though it is actually observed, and second, even when ∆Gγε

MSis negative, its

magnitude is in many cases very small and possibly insufficient to account for the strain energy oftransformation.

There are two ways in which these results might be understood. The first is that the experimentalmeasurements of MS temperatures are faulty, but a detailed examination of the original sources ofinformation indicated that any error in MS is much smaller than required to explain the sign andmagnitude of the free energy change in cases where ∆Gγε

MS≫ 0. Nevertheless, we discuss later in

this paper, our own experimental data designed to assess experimental error.

The second and more likely explanation is that the database which forms the basis of the thermo-dynamic calculations described in section 3 is insufficiently populated to represent ε–martensite inconcentrated alloys and at the relatively low temperatures involved. First principles calculationsbased on electron theory can be used to check this second explanation, but the calculations areexpensive to conduct so a particular alloy which indicated a large positive ∆Gγǫ = Gε−Gγ in spiteof the observation of martensite was selected for study.

The conventional unit cells of austenite (FCC) and ε (HCP) can both be represented by the stackingof layers of close–packed planes, with each layer containing 4 atoms with a total of 24 atoms, andhence six layers, with both phases treated as being non–magnetic. The lattice parameters (a, c) ofthe conventional hexagonal unit cell is then determined as a =

√2aγ and c = 2

√3aγ . The lattice

parameter of austenite is applied as aγ = 3.59A[80]. The only difference between the FCC andHCP forms is then the stacking sequence which is ABCABC and ABABAB, respectively. The alloycomposition is created by an appropriate substitution of Fe atoms with five Mn, two Si and two Cratoms, Fig 3.

The Kohn-Sham equation was solved self-consistently in terms of the total energy all-electronfull-potential linearised augmented plane-wave method [81, 82] by using the generalised gradientapproximation for the exchange-correlation potential. The integrations over the three dimensionalBrillouin zone (3D-BZ) were calculated by the tetrahedron method over a 7×7×5 Monkhorst-Packmesh [83], which corresponds to 123 k-points inside the irreducible wedge of 3D-BZ. The degree of

3

precision was obtained by considering a plane-wave cutoff up to 21Ry, which corresponds to about3245 linearised augmented plane-waves per each k-point and spin. The wave functions, the chargedensities, and the potential were expanded with l < 8 lattice harmonics inside each muffin-tinsphere with a radius of 2.20 a.u. for Fe,Mn,Si and Cr. The density and potential in the interstitialregion were depicted by using a star-function cutoff at 340Ry. Self-consistency was assumed whenthe root-mean-square distances between the input and output total charges were not more than2.0 × 10−3 electrons/a.u.3 The sphere radii and Kmax within the whole lattice spacing range werekept constant, to keep the same degree of convergence for all the lattice constants studied.

The transformation energies at 0 K and zero pressure were calculated to give ∆Gγε as−5.57 kJ mol−1

and −3.49 kJ mol−1 for the transformation in pure iron and 15Fe-5Mn-2Si-2Cr alloy respectively,where the alloy composition is expressed in terms of the number of atoms out of a total of 24 atoms.The value for pure iron is remarkably consistent with the −5.45 kJ mol−1 reported in [84] for oneatomsphere of pressure and 0K. based on a thermodynamic assessment. This calculation proves theneed for better thermodynamic data for use in software such as Thermocalc or MTDATA. It is ourintention in the future to undertake a major programme of first principles calculations, includinglattice parameter calculations (as opposed to the fixed parameters assumed here) in order to assessand enhance the thermodynamic database for the ε phase.

Given the difficulties with the thermodynamic data, the best that can be done is focus on those alloyswhere the critical driving force ∆Gγε

MS< 0 (i.e., a reduction in free energy). Given the availability

of data from binary Fe–Mn alloys with large differences in the manganese concentrations, thedependence of ∆Gγε

MSon Mn has been derived as illustrated in Fig. 4a. Calculations carried out to

estimate MS assuming that all other solutes influence only ∆Gγε are shown in Fig. 4b. Note thatwe do not understand the functional dependence illustrated in Fig. 4a, and that the accuracy ofthe predictions illustrated in Fig. 4b is not impressive even when the analysis is limited to thosecases where the transformation is accompanied by a reduction in free energy.

4 Experiments

The purpose of the work presented here was to check the level of experimental error expected inmeasuring the start temperature for ε, given that the volume change of transformation might insome cases be rather small [85, 86]. A set of six alloys showing a variation in manganese and siliconconcentrations, was prepared as 300 g melts, which were cast and vacuum sealed. They were thenhomogenised for 2 days at 1473 K, after which their chemical compositions were measured as listedin Table 2. Cylindrical dilatometer samples 5mm diameter and 10mm long were machined andstudied using a BAHR DIL805 dilatometer. The samples were heated at 2K s−1 in a vacuum to873K for 1min, and then quenched at 10K s−1 using argon gas to room temperature.

The results of dilatometric experiments are presented in Fig. 5. A method exists which enablessuch data to be interpreted objectively, so that any user analysing the same data should obtain anidentical transformation–start temperature [87]. The technique defines the first onset of transfor-mation to be that at which a critical strain is achieved relative to the thermal contraction of theparent phase. In the present work the critical strain has been taken as 1/100 of the total trans-formation strain determined at ambient temperature for the 16Mn 0Si alloy, equal to −4.6× 10−5.

4

Note that although this small offset should be greater than the noise in the data, it is an arbitrarybut reproducible value which is used for all the alloys. It is akin to the arbitrary, small strain usedin defining the proof strength in a gradually yielding tensile test. Optical metallography was usedto confirm the existence of ǫ–martensite and two representative examples are presented in Fig. 6.

Using this method, it is clear from Table 2 that with one exception where the volume change ontransformation is rather small, the uncertainties in the determination of martensite–start temper-atures are small and cannot explain the major discrepancies found in the ∆Gγε values calculatedusing existing thermodynamic databases.

5 Neural Network

The most general method of regression analysis is the neural network, because it is able to capturenon–linear and non–periodic functions of immense complexity without bias on the form of thefunction. Comprehensive details of this method have been described elsewhere [88–91] and henceare not reproduced here except when the information is necessary to reproduce the work.

To create a network which is not too simple, nor so complex that it models the noise in the infor-mation, the data were partitioned at random into approximately equal training and test sets. Theformer was used to create the models and the latter to test their ability to generalise. Once theappropriate level of complexity is achieved, the entire data can be used to retrain the network with-out changing its configuration. The results, having gone through these procedures, are illustratedin Fig. 7 and show that the optimised network performs well on the unseen test data.

We now show an example to illustrate the non–linear capability of the neural network, whichis consistent with expectations from physical metallurgy but would not be captured by a linearregression equation. The Neel temperature TN of austenite is raised almost linearly by the additionof manganese [38] and this has an enhanced effect on suppressing the εmartensite–start temperatureif the latter is below TN [92]. That this phenomenon is correctly represented by the neural networkis illustrated in Fig. 8.

6 Austenite Grain Size Effect

It has been shown recently [93] that the dependence of MS on the austenite grain size during theγ → α′ transformation can be explained quantitatively on the basis of Fisher’s original suggestion[94] that the number of plates per unit volume needed in order to obtain a detectable fraction ofmartensite increases as the austenite grain volume (Vγ) decreases, because the plate size and hencethe volume transformed per plate is reduced with Vγ . This leads to an expression [93]:

MoS − T =

1

bln

[

1

aVγ

{

exp

(

− ln(1− f)

m

)

− 1

}

+ 1

]

(3)

whereMS → MoS as Vγ → ∞, and f is the fraction of martensite, with the volume measured in mm3

the term a can be set to unity, m is the aspect ratio of martensite plates, and b is a constant. This

5

relationship enables the amount of martensite to be calculated as a function of undercooling belowMS with the latter defined by the undercooling needed to achieve a detectable fraction fMS

. Whenthe temperature T is sufficiently below Mo

S the equation reduces to the classical Koistinen andMarburger relation [95] which is independent of grain size and expressed here in the terminologyof equation 3:

ln{1− f} = −m ln Vγ −mb(MoS − T ) (4)

where Koistinen and Marburger obtained mb = 0.011K−1 for the γ → α′ transformation. The tworelationships in fact only differ in the narrow temperature range at the beginning of transformation.

There exist three sets of experiments where ε–martensite has been studied as a function of theaustenite grain size [29, 39, 62]. Fig. 9a shows that all three sets of data can be used to deriveb = 0.33, and taking the aspect ratio of ε as m = 0.03 [39], mb = 0.01K−1, a value which isremarkably similar to the original due to Koistinen and Marburger for α′ martensite. This maywell be a coincidence but the fact that these values are not dramatically different neverthelessinspires confidence in the analysis. The values of Mo

S are also obtained from the intercepts on thevertical axes of Fig. 9a. The final results are plotted in Fig. 9b, showing that all the data can berationalised in terms of equation 3. Jiang et al. [62] in their work concluded that there is no grainsize dependence of MS for ε, but Fig. 9b shows that this is because the grain size was not variedsufficiently in their experiments.

7 Conclusions

The thermodynamic method used so successfully in predicting the MS temperature for the γ → α′

transformation cannot be implemented fully for ε because of the availability of thermodynamicdata. A reasonable assumption can be made that it is the dataset for ε which is lacking since theγ phase is well characterised. This is partly supported by a limited calculation done using firstprinciples, but to do this generally is an expensive option and the focus perhaps needs to be onspecific cases of technological interest. A limited number of experiments on six combinations ofmanganese and silicon supports the conclusion that the thermodynamic data are wanting, and theproblem does not lie in potential inaccuracies in the measurement of martensite–start temperatures.

A linear regression equation has been derived based on a large experimental dataset accumulatedfrom the published literature, as a rough method for estimating the γ → ε martensite–start tem-peratures. This is unable to capture the non–linear effects apparent in the experimental data,for example the dependence on the manganese concentration. Therefore, a corresponding neuralnetwork model has also been created, which should be a better tool than the linear method.

It has been demonstrated that the austenite grain size dependence of the start–temperature forε martensite can be rationalised in terms of existing theory which is based on the fact that theminimum detectable quantity of transformation, which defines MS , is a function of the grain size.

The neural network models, thermodynamic calculations and the full set of compiled data can bedownloaded from [79].

6

Acknowledgments

We acknowledge Professor Nack Joon Kim for the provision of laboratory facilities at GIFT, andsupport from POSCO through the Steel Innovation Programme. The authors are also gratefulfor support from the World Class University Programme of the National Research Foundation ofKorea, Ministry of Education, Science and Technology, project number R32–2008–000–10147–0.

References

[1] L. Kaufman, M. Cohen: Progress in Metal Physics 7 (1958) 165–246.

[2] G. B. Olson, M. Cohen: Metallurgical Transactions A 7A (1976) 1897–1923.

[3] J. W. Christian: Thermodynamics and kinetics of martensite: in: G. B. Olson, M. Cohen(Eds.), International Conference on Martensitic Transformations ICOMAT ’79: 1979: pp.220–234.

[4] L. Kaufman, S. V. Radcliffe, M. Cohen: Thermodynamics of the bainite reaction: in: V. F. Za-ckay, H. I. Aaronson (Eds.), Decomposition of Austenite by Diffusional Processes: Interscience,New York, USA, 1962: pp. 313–352.

[5] Y. Imai, M. Izumiyama, M. Tsuchiya: Scientific Reports: Research Institute of Tohoku Uni-versity A17 (1965) 173–192.

[6] T. Bell, W. S. Owen: Trans. Metall. Soc. AIME 239 (1967) 1940–1949.

[7] H. K. D. H. Bhadeshia: Metal Science 15 (1981) 175–177.

[8] H. K. D. H. Bhadeshia: Metal Science 15 (1981) 178–180.

[9] H. Chang, T. Y. Hsu: Acta Metallurgica 34 (1986) 333–338.

[10] G. Ghosh, G. B. Olson: Acta Metallurgica and Materialia 42 (1994) 3361–3370.

[11] J. Wang, P. J. van der Wolk, S. van der Zwaag: Materials Transactions JIM 41 (2000) 769–776.

[12] G. Ghosh, G. B. Olson: Journal of Phase Equilibria 22 (2001) 199–207.

[13] U. of Cambridge, NPL: Materials Algorithms Project,www.msm.cam.ac.uk/map/mapmain.html

[14] O. Grassel, L. Kruger, G. Frommeyer, L. W. Meyer: International Journal of Plasticity 16(2000) 1391–1409.

[15] G. Frommeyer, U. Brux, P. Neumann: ISIJ International 43 (2003) 438–446.

[16] D. Embury, O. Bouaziz: Annual Reviews in Materials Science 40 (2010) 213–241.

[17] A. Sato, E. Shishima, Y. Yamaji, T. Mori: Acta Metallurgica 32 (1984) 539–547.

[18] J. Li, C. M. Wayman: Materials Characterization 32 (1994) 215–227.

7

[19] Y. Tomota, T. Maki: Materials Science Forum 327–328 (2000) 191–198.

[20] A. Dogan, T. Ozer: Canadian Metallurgical Quarterly 44 (2005) 555–561.

[21] Q. X. Dai, X. N. Cheng, Y. T. Zhao, X. M. Luo, Z. Z. Yuan: Materials Characterization 52(2004) 349–354.

[22] S. H. Baik, J. C. Kim, K. K. Jee, M. C. Shin, C. S. Choi: ISIJ International 37 (1997) 519–522.

[23] M. Sade, K. Halter, E. Hornbogen: Journal of Materials Science Letters 9 (1990) 112–115.

[24] T. Liu, Z. T. Zhao, R. Z. Ma: Phase Transitions 69 (1999) 425–428.

[25] N. van Caenegem, L. Duprez, K. Verbeken, D. Segers, Y. Houbaert: Materials Science &Engineering A 481–482 (2008) 183–189.

[26] S. Takaki, T. Furuya, Y. Tokunaga: ISIJ International 30 (1990) 632–638.

[27] Y. K. Lee, C. S. Choi: Metallurgical & Materials Transactions A 31 (2000) 355–360.

[28] Y. Tomota, M. Stum, J. W. Morris Jr.: Metallurgical Transactions A 17 (1986) 537–547.

[29] J. H. Jun, C. S. Choi: Materials Science & Engineering A 257 (1998) 535–556.

[30] Y. Tomota, Y. Morioka, W. Nakagawara: Acta Materialia 46 (1998) 1419–1426.

[31] Y. K. Lee, J. H. Jun, C. S. Choi: Scripta Materialia 35 (1996) 825–830.

[32] Y. K. Lee, J. H. Jun, C. S. Choi: ISIJ International 37 (1997) 1023–1030.

[33] J.-H. Jun, D.-K. Kong, C.-S. Choi: Materials Research Bulletin 33 (1998) 1419–1425.

[34] J. H. Jun, C. S. Choi: Scripta Materialia 38 (1998) 543–549.

[35] J. H. Jun, C. S. Choi: Materials Science & Engineering A 252 (1998) 133–138.

[36] S. Cotes, M. Sade, A. F. Guillermet: Metallurgical and Materials Transactions A 26 (1995)1957–1969.

[37] J. T. Lenkkeri, J. Levoska: Philosophical Magazine A 48 (1983) 749–758.

[38] H. Umebayashi, Y. Ishikawa: Journal of the Physical Society of Japan 21 (1966) 1281–1294.

[39] S. Takaki, H. Nakatsu, T. Tokunaga: Materials Transactions JIM 34 (1993) 489–495.

[40] S. Cotes, A. F. Guillermet, M. Sade: Journal of Alloys and Compounds 278 (1998) 231–238.

[41] I. Y. Georgiyeva, N. A. Sorokina, V. I. Gal’tsova: Physics of Metals and Metallography 49(1981) 178–181.

[42] K. Ishida, T. Nishizawa: Transactions of the Japan Institute of Metals 15 (1974) 225–231.

[43] A. P. Gulyaev, T. F. Volynova, I. Y. Georgiyeva: Metals Science and Heat Treatment 20 (1978)179–182.

[44] A. R. Troiano, F. T. McGuire: Trans. ASM 31 (1943) 340–364.

8

[45] I. N. Bogachev, L. S. Malinov: Physics of Metals and Metallography 14 (1962) 828–833.

[46] I. N. Bogachev, V. F. Yegolayev, G. Y. Zvigintseva, L. V. Zhuravel: Physics of Metals andMetallography 28 (1968) 885–888.

[47] M. Eskil, E. Kanaca: Computational Materials Science 43 (2008) 774–784.

[48] A. Druker, A. Baruj, J. Malarria: Materials Characterization 61 (2010) 603–612.

[49] C. H. Yang, H. C. Lin, K. M. Lin: Materials Science & Engineering A 518 (2009) 139–143.

[50] K. Tsuzaki, S. Fukasaku, Y. Tomota, T. Maki: Trans. JIM 32 (1991) 222–228.

[51] H. Otsuka, H. Yamada, T. Maruyama, H. Tanahashi, S. Matsuda, M. Murakami: ISIJ Inter-national 30 (1990) 674–679.

[52] M. Fujita, I. Uchiyama: Tetsu–to–Hagane 60 (1974) 525–539.

[53] A. A. H. Hamers, C. M. Wayman: Scripta Metallurgica and Materialia 25 (1991) 2723–2728.

[54] P. Donner, E. Hornbogen, M. Sade: Journal of Materials Science 8 (1989) 37–40.

[55] A. Baruj, S. Cotes, M. Sade, A. F. Guillermet: Journal de Physique Colloque 5 (1995) C8373–378.

[56] M. Acet, T. Schneider, B. Gehrmann, E. F. Wassermann: Journal de Physique Colloque 5(1995) C8 379–384.

[57] K. K. Jee, W. Y. Jang, S. H. Baik, M. C. Shin, C. S. Choi: Journal de Physique Colloque 5(1995) C8 385–390.

[58] T. Bouraoui, A. van Neste, B. Dubois: Journal de Physique Colloque 5 (1995) C8 403–408.

[59] D. P. Dunne, H. Li: Journal de Physique Colloque 5 (1995) C8 415–420.

[60] Y. Tomota, K. Yamaguchi: Journal de Physique Colloque 5 (1995) C8 421–426.

[61] M. Andersson, J. A. gren: Journal de Physique Colloque 5 (1995) C8 457–462.

[62] B. H. Jiang, X. Qi, W. Zhou, T. Y. Hsu: Scripta Materialia 34 (1996) 771–773.

[63] L. J. Rong, D. H. Ping, Y. Y. Li, C. X. Shi: Scripta Materialia 32 (1995) 1905–1909.

[64] S. Chen, C. Y. Chung, C. Yan, T. Y. Hsu: Materials Science & Engineering A 264 (1999)262–268.

[65] H. Li, D. Dunne, N. Kennon: Materials Science & Engineering A 273–275 (1999) 517–523.

[66] X. Wu, T. Y. Hsu: Materials Characterization 45 (2000) 137–142.

[67] Y. Wen, N. Li, M. Tu: Scripta Materialia 44 (2001) 1113–1116.

[68] W. Zhou, B. Jiang, X. Qi, T. Y. Hsu: Scripta Materialia 39 (1998) 1483–1487.

[69] Y. H. Wen, M. Yan, N. Li: Scripta Materialia 50 (2004) 441–444.

[70] Z. Wang, J. Zhu: Wear 256 (2004) 66–72.

9

[71] B. C. Maji, M. Krishnan: Scripta Materialia 48 (2003) 71–77.

[72] Y. S. Zhang, X. Lu, X. Tian, Z. Qin: Materials Science & Engineering A 334 (2002) 19–27.

[73] Y. H. Wen, W. L. Xie, D. Li: Materials Science & Engineering A 457 (2007) 334–337.

[74] V. G. Gavriljuk, V. V. Bliznuk, B. D. Shanina, S. P. Kolesnik: Materials Science & EngineeringA 406 (2005) 1–10.

[75] K. Yamaguchi, Y. Morioka, Y. Tomota: Scripta Materialia 35 (1996) 1147–1152.

[76] C. L. Li, D. J. Cheng, Z. H. Jin: Scripta Materialia 35 (1996) 1147–1152.

[77] J. H. Yang, H. Chen, C. M. Wayman: Metallurgical Transactions A 23 (1992) 1431–1437.

[78] Y. Tomota, W. Nakagawara, K. Tsuzaki, T. Maki: Scripta Materialia 26 (1992) 1571–1574.

[79] H. S. Yang: Data for epsilon martensite–start temperatures insteels, http://www.msm.cam.ac.uk/map/steel/programs/epsilon.Ms.html andhttp://cml.postech.ac.kr/2011/epsilon.zip (2011).

[80] A. Lambert-Perlade: Rupture par clivage de microstructures d’aciers bainitiques obtenues enconditions de soudage: Ph.D. thesis: Ecole de Mines de Paris: Paris, France (2001).

[81] E. Wimmer, H. Karkauer, M. Weinert, A. J. Freeman: Physical Review B 24 (1981) 864–875.

[82] M. Weinert, E. Wimmer, A. J. Freeman: Physical Review B 26 (1982) 4571–4578.

[83] H. J. Monkhorst, J. D. Pack: Physical Review B 13 (1976) 3865–3868.

[84] L. Kaufman, E. V. Clougherty, R. J. Weiss: Acta Metallurgica 11 (1963) 323–335.

[85] J. W. Brooks, M. H. Loretto, R. E. Smallman: Acta Metallurgica 27 (1979) 1829–1838.

[86] J. W. Brooks, M. H. Loretto, R. E. Smallman: Acta Metallurgica 27 (1979) 1839–1847.

[87] H.-S. Yang, H. K. D. H. Bhadeshia: Materials Science and Technology 23 (2007) 556–560.

[88] D. J. C. MacKay: Neural Computation 4 (1992) 448–472.

[89] D. J. C. MacKay: Neural Computation 4 (1992) 415–447.

[90] H. K. D. H. Bhadeshia: Statistical Analysis and Data Mining 1 (2009) 296–305.

[91] H. K. D. H. Bhadeshia, R. C. Dimitriu, S. Forsik, J. H. Pak, J. H. Ryu: Materials Science andTechnology 25 (2009) 504–510.

[92] M. Palumbo: CALPHAD 32 (2008) 693–708.

[93] H. S. Yang, H. K. D. H. Bhadeshia: Scripta Materialia 60 (2009) 493–495.

[94] J. C. Fisher, J. H. Hollomon, D. Turnbull: Metals Transactions 185 (1949) 691–700.

[95] D. P. Koistinen, R. E. Marburger: Acta Metallurgica 7 (1959) 59–60.

10

Table 1: Dataset statistics, rounded off to significant figures after the decimal point, for a total of328 separate measurements as described in the text. The concentrations of solutes are in wt%.

Minimum Maximum Average Standard deviation

C 0 0.35 0.02 0.05

Mn 11.2 35.9 22.2 6

Ni 0 6.8 0.47 1.5

Cr 0 13.7 1.5 3.2

Al 0 5 0.16 0.8

Si 0 7.1 2.1 2.5

Mo 0 4.46 0.03 0.3

Co 0 8 0.29 1.2

Cu 0 3.1 0.03 0.25

Nb 0 1.21 0.01 0.08

Ti 0 1.72 0.01 0.12

V 0 2.2 0.01 0.15

W 0 4.48 0.03 0.31

MS / K 167 467 352 60

11

Table 2: Alloy compositions and measured MS temperatures

Alloy designation Mn / wt% Si / wt% MS / K

16Mn 0 Si 15.8 0.0 410± 3

16Mn 3 Si 15.6 2.7 437± 7

16Mn 6 Si 16.0 5.4 422± 1

25Mn 0 Si 24.8 0.1 < 293

25Mn 3 Si 25.3 2.8 343± 2

25Mn 6 Si 25.0 5.2 441± 1

12

Figure 1: The ε–martensite MS temper-atures estimated using equation 2, versusmeasured values.

Figure 2: The calculated free energy changeaccompanying the formation of ε–martensiteat the measured MS temperature. Noticethat the scales above and below the ab-scissa are different. The samples for which∆Gγε

MS≥ 0 are generally those which have

large total solute concentrations, for exam-ple, Fe–26Mn–5Cr–6Si wt%.

13

(a) (b)

Figure 3: The supercells used in the first–principles calculations.

(a) (b)

Figure 4: Thermodynamic method applied only to those alloys for which ∆GγεMS

< 0 using currentthermodynamic databases. (a) Dependence of ∆Gγε

MSon the manganese concentration. (b) An

illustration of the accuracy with which predictions can be made assuming that the critical drivingforce at MS varies only with the Mn concentration.

14

Figure 5: Heating and cooling dilatomet-ric data for all of the experimental alloys.Note that there is a contraction when ε–martensite forms from austenite. The datahere are presented with a compressed verti-cal axis for the sake of brevity, but the full,high–resolution set is available on [79].

(a) (b)

Figure 6: Optical micrographs showing ε martensite. (a) 16Mn 0Si alloy. (b) 25Mn 3Si alloy.

15

(a) (b)

Figure 7: Illustration of the fit achieved with a neural network of optimum complexity. The errorbars represent ±1σ modelling uncertainty. (a) Data used to create the network. (b) Unseen dataused to test the network.

(a) (b)

Figure 8: Variation in the martensite–start temperature in Fe–Mn alloys as a function of themanganese concentration. (a) Calculated using neural network. (b) Measured values from publishedwork, together with the calculated curve from (a). The Neel temperature (TN ) data are from [38].

16

(a) (b)

Figure 9: Analysis of the austenite grain size dependence of MS for ε–martensite. The circles,crosses and squares are data from [29], [39] and [62] respectively. (a) Linear regression to derive band Mo

S . (b) Comparison between measured data and curve calculated using equation 3.

17